1 Behaviour of hollow pultruded GFRP square beams with different shear span-to-depth ratios Journal: Manuscript ID: Draft Manuscript Type: Original Manuscript Date Submitted by the Author: n/a Complete List of Authors: Muttashar, Majid; University of Southern Queensland, Centre of Excellence in Engineered Fibre Composites Karunasena, Warna; University of Southern Queensland, Centre of Excellence in Engineered Fibre Composites Manalo, Allan; University of Southern Queensland, Centre of Excellence in Engineered Fibre Composites Lokuge, Weena; University of Southern Queensland, Centre of Excellence in Engineered Fibre Composites Keywords: Abstract: Pultruded sections, fibre composites, elastic properties, characterization, shear span, full-scale testing It is important to determine accurately the elastic properties of fibre reinforced polymer (FRP) composites material, considering that their member design is often governed by deflection rather than strength. In this study, the elastic properties of the pultruded glass FRP (GFRP) square sections were evaluated firstly using full-scale with different shear span to depth (a/d) ratios and tested under static four-point bending. Back calculation and simultaneous methods were then employed to evaluate the flexural modulus and shear stiffness and were compared with the results of the coupon tests. Secondly, the full-scale beams were tested up to failure to determine their capacity and failure mechanisms. Finally, prediction equations describing the behaviour of the pultruded GFRP square beams were proposed and compared with the experimental results. The results indicate that the back calculation method gives more reliable values of elastic properties of GFRP profiles. In addition, the behaviour of the beams is strongly affected by the a/d ratios. The shear was found to have a significant contribution on the behaviour of beams with lower a/d ratios while the flexural stress played a major part for higher a/d ratios. The proposed equation, which accounts for the combined effect of the shear and flexural stresses, reasonably predicted the failure load of pultruded GFRP square beams.
2 Page of
3 Page of Research paper Behaviour of hollow pultruded GFRP square beams with different shear span-to-depth ratios (Title contains words) Running headline: Behaviour of Hollow Pultruded GFRP square Beams with Different Shear Span-to-Depth Ratios ( characters) by Majid Muttashar,, Warna Karunasena, Allan Manalo,* and Weena Lokuge Centre of Excellence in Engineered Fibre Composites (CEEFC), School of Civil Engineering and Surveying, University of Southern Queensland, Toowoomba, 0, Australia Department of Civil Engineering, College of Engineering, University of Thi Qar, Iraq. Submitted to Corresponding Author * : Allan Manalo Senior Lecturer in Civil Engineering (Structural) Centre of Excellence in Engineered Fibre Composites (CEEFC), School of Civil Engineering and Surveying, University of Southern Queensland, Toowoomba, Queensland 0, Australia Manuscript summary: Total pages (including -page cover) Number of figures Number of tables 0
4 Page of Behaviour of hollow pultruded GFRP square beams with different shear span-to-depth ratios Abstract Majid Muttashar,, Warna Karunasena, Allan Manalo,* and Weena Lokuge It is important to determine accurately the elastic properties of fibre reinforced polymer (FRP) composites material, considering that their member design is often governed by deflection rather than strength. In this study, the elastic properties of the pultruded glass FRP (GFRP) square sections were evaluated firstly using full-scale with different shear span to depth (a/d) ratios and tested under static four-point bending. Back calculation and simultaneous methods were then employed to evaluate the flexural modulus and shear stiffness and were compared with the results of the coupon tests. Secondly, the full-scale beams were tested up to failure to determine their capacity and failure mechanisms. Finally, prediction equations describing the behaviour of the pultruded GFRP square beams were proposed and compared with the experimental results. The results indicate that the back calculation method gives more reliable values of elastic properties of GFRP profiles. In addition, the behaviour of the beams is strongly affected by the a/d ratios. The shear was found to have a significant contribution on the behaviour of beams with lower a/d ratios while the flexural stress played a major part for higher a/d ratios. The proposed equation, which accounts for the combined effect of the shear and flexural stresses, reasonably predicted the failure load of pultruded GFRP square beams. Centre of Excellence in Engineered Fibre Composites (CEEFC), School of Civil Engineering and Surveying, University of Southern Queensland, Toowoomba, 0, Australia Department of Civil Engineering, College of Engineering, University of Thi Qar, Iraq. * Corresponding author: Allan Manalo, Centre of Excellence in Engineered Fibre Composites (CEEFC), School of Civil Engineering and Surveying, University of Southern Queensland, Toowoomba, 0, Australia
5 Page of Keywords: Elastic properties, characterization, shear, flexural, failure load, GFRP beams Introduction Fibre reinforced polymer (FRP) composites emerged as a promising material to satisfy the increasing demand for better performing and more durable civil infrastructures. Recently, FRP composites have been used in bridges, because of their high stiffness, strength-to-weight ratios, corrosion resistance and durability. In addition to these superior properties, the process of producing FRP sections allows the designer to specify different material properties for different parts of the cross section. Nevertheless, the use of these advanced materials in structural applications is constrained due to limited knowledge on their material properties and structural behaviour. Therefore it is of paramount importance to investigate the properties of pultruded FRP sections so that they can be broadly utilised in structural applications. A number of micromechanical simulations have already been developed to predict the properties of pultruded beams such as flexural and shear modulus -. The mechanical properties estimated using these models showed a good correlation with the experimental results. However, the models require accurate information on the processing details of the FRP profiles such as individual properties of fibres and resin, the fibre volume fraction and the composition of the laminates. Therefore, the use of these models as a design tool for structural purposes is likely to complicate the process. Thus, several researchers investigated coupon specimens to determine the effective mechanical properties of the composites and used these properties to predict the behaviour of full scale pultruded FRP profiles,. Manaloet al. 0 mentioned that there are limited test methods and equipment to characterise the properties of thick FRP composites by using the results of coupon tests. Moreover, the limited dimensions in the transverse direction of the majority of the pultruded GFRP sections added a new obstacle to the applicability of available test standards. The complex internal
6 Page of structure of composites and/or the variation of its mechanical properties within the element itself warrant testing of full scale sections to obtain realistic design properties. Guadeset al. conducted an experimental investigation to characterise the mechanical properties of square pultruded sections (00 mm x 00 mm) using both coupon and full scale specimens. Although, there was a good agreement between the coupon and full-scale results for single span beams, the effect of shear deformation on the behaviour of the pultruded profiles was neglected as the beam considered in sufficiently long. Bank indicated that the effect of shear on thin walled FRP sections is very significant especially for shorter beams and should be considered in determining the elastic properties of composite material. In support of this, Bank and Neto and Rovere conducted experiments using full-scale sections to determine the flexural (E) and shear (G) modulus of FRP composite beams. In both situations, three point bending tests were used to characterise the behaviour of beams with different spans. Even though same test procedure and almost similar section properties were used in both research, there was a huge difference between the calculated E/G ratios as Bank determined the elastic modulus based on Timoshenko Beam Theory while Neto and Rovere used the graphical (simultaneous) test method. Mottram stated that the sensitivity of the graphical method in determining the slope (of the regression line through the data points) can lead to a significant change in the E and G calculations. As a result, there is a need to revisit the graphical method used to find the flexural and shear modulus. To the authors knowledge, there are very limited experimental studies conducted to determine the structural properties of full scale FRP composite beams made of vinyl ester resin with E-glass fibre reinforcement oriented in different directions. In this study, hollow pultruded GFRP square beams with different shear span-to-depth (a/d) ratios were tested using static four point bending configuration. Graphical (simultaneous) and back
7 Page of calculation methods were used to calculate the E and G and compared with the results of the coupon test. In addition, the effect of a/d ratio on the strength and failure behaviour of the GFRP beams was analysed. Based on the experimental results of this research, a simplified prediction equation to obtain the failure load of the GFRP beams was proposed with due consideration given to the effect of a/d ratio. These predicted failure loads are then compared with the experimental results. Determination of flexural and shear modulus (Beam Theory) The relatively low elastic modulus of GFRP leads to designs being governed by deflection and buckling limitations, instead of strength,. In addition, the anisotropic nature of the FRP composites results in low shear modulus to longitudinal elastic modulus ratio. Accordingly, the contribution of shear deformation in the total deformation becomes significant and should be considered in designing composite structures,,. This shear contribution can be theorised by using Timoshenko beam theory. This theory incorporates shear deformation of thin walled composite sections in deflection and investigates its effect in a quantitative manner in order to reliably determine the E and G for the pultruded FRP section. In this method the controlling equations are: = () + = where I is the second moment of area, is the bending slope, M is the bending moment, δ is the total deflection, V is the shear force and A is the cross- sectional area. The shear coefficient K is a constant which accounts for the shear distribution over the beam cross section. For homogenous box profile, K can be calculated using the equation recommended by Bank : K= () ()
8 Page of where υ, G and E refer to the longitudinal Poisson s ratio, shear modulus and elastic modulus, respectively of the section. By solving equations and for the case of four- point load bending with the load applied at a distance (a) from the support point (a=l/ in this case, where L is the beam span), the total deflection can be obtained as follows: = + where P is the total applied load, EI is the flexural stiffness and KGA is the shear stiffness. Two techniques are commonly used to calculate EI and KGA by using the above equation. The first technique is called back calculation method (BCM) which was based on the Bernoulli equation to determine the EI from the strain readings on the outer flange surfaces at mid-span (in the constant moment region): = where c is the distance from the neutral axis to the outermost fibre, and ε is the measured strain. After EI is calculated, Equation can be used to back calculate KGA. The second technique is referred to as simultaneous method (SM) where at least two different spans should be investigated experimentally. Each test produces a data set for load, deflection and span. These three terms are known in Equation with EI and KGA as two unknowns. For better interpretation of the method, Equation is divided throughout by PL/A as follows: = + This represents a straight line, with (L/r) being the independent variable on the horizontal axis and Aδ/PL being the dependent variable on the vertical axis. Herein, r is the radius of gyration of the section defined by =. By plotting the variable () () () against, the elastic modulus can be found from the slope of the straight line and the shear modulus from the intercept on the vertical axis:
9 Page of = = Experiment program Material properties Pultruded GFRP square sections ( mm x mm x. mm thickness) produced by Wagner s Composite Fibre Technologies (WCFT), Australia were used in this study. These sections are made from vinyl ester resin with E-glass fibre reinforcement. The density of these pultruded profiles is 0 kg/m. As per standard ISO, the burnout test revealed an overall glass content of % by weight in these profiles. The stacking sequence of the plies is [0 0 /+ 0 /0 0 /- 0 /0 0 /- 0 /0 0 /+ 0 /0 0 ], where the 0 o direction aligns with the longitudinal axis of the tube. Table shows the mechanical properties of the pultruded sections determined from coupon tests. Table. Mechanical properties from coupon test Characterization of elastic properties for pultruded sections Following the methodology proposed by Bank, GFRP pultruded profiles with three different a/d ratios were tested under static four - point bending. The details of the tested specimens are listed in Table. The load was applied at the third points of the span and shear span to total length (a/l) was maintained at / for all tests. Figure shows the schematic illustration of the test set-up and the tests were conducted according to ASTM D. A 00 kn capacity servo hydraulic testing machine was used with a loading rate of mm/min. All specimens were tested only up to approximately % of the failure load to ensure that the beams are still in the elastic range. Strain gauges (PFL---L-0) of mm length were attached to the bottom face at the mid-span of the specimens. Laser displacement transducer () ()
10 Page of was used to measure the mid-span deflection. The applied load and the deflection of the loading ram were recorded using the Systems 000 data acquisition system. Table. Details of the specimens tested for the elastic properties Figure. Experimental set-up for characterisation of elastic properties. Behaviour of hollow pultruded GFRP composite beams Hollow GFRP pultruded sections with four different a/d ratios were tested up to failure under static four point bending test. In contrast to section., the load was applied at the two points with a load span equal to 00 mm. The constant load span was used to keep the upper face of the section under same condition for all specimens and to take account of the limitation on the length of the test frame. Vertical supports were provided to prevent lateral buckling. The details of the tested specimens are listed in Table. Figure shows the experimental set up. A 00 kn capacity universal machine was used for applying the load. Steel plates were provided at the support and loading points to minimise indentation failure. Table. Details of the specimens tested for the behaviour of GFRP beams Figure. Experimental setup for the behaviour of GFRP beams. Experimental results and observations The experimental results for the elastic properties and the behaviour of full scale beams are discussed in this section. Elastic properties of GFRP sections E and G using back calculation method. The load versus deflection curves for all specimens are shown in Figure. Linear elastic behaviour up to kn can be observed from these. The variations of E and KGA with load for all specimens are shown in Figures to. From these curves, it can be seen that these parameters start at a high value but reduce with increasing load. In order to minimise the errors that might have occurred due to deflection
11 Page 0 of measurements in this study, EI and KGA were computed from the average of several points spaced within a range of L/00 to L/00 deflection as suggested by Hayes and Lesko. The average calculated values of E and KGA from the BCM are summarized in Table. In this table, a numerical value for the moment of inertia has been used. The shear modulus G is separated from KGA using the k determined from equation () and the nominal cross section area of the beam. The average value of E was. GPa which is % higher than the coupon test results. The higher flexural modulus obtained from the full section compared with the coupon specimens can be related to the continuity of ± o fibres along the length of the pultruded beams. In addition, the shear modulus value of GPa is comparable with the value suggested by Mottram for a standard GFRP pultruded profile. Figure. Load deflection relationship for GFRP beams. Figure. Elastic modulus (E) and Shear stiffness (KGA) versus Load for a/d =. Figure. Flexural Modulus (E) and Shear Stiffness (KGA) versus Load for a/d =. Figure. Flexural Modulus (E) and Shear Stiffness (KGA) versus Load for a/d =. Table. Summary of average E and KGA for each span for GFRP beam testing (BCM) E and G using simultaneous method. In order to determine the elastic properties E and G, a graph for Aδ/PL versus (L/r) was plotted as shown in Figure. A linear regression was used to obtain the slope, intercept and the coefficient of correlation, which are also shown in the figure. The E and G values were then calculated using equations and, respectively. The calculated E in this method is. GPa which is higher than the coupon test results by about %. In contrast, G is. GPa which is less than the average value for standard pultruded profiles by about %. Figure. Typical graph to determine E and KG using simultaneous method. Behaviour of hollow pultruded GFRP composite beams
12 Page of Load-deflection behaviour. Figure shows the load - deflection curves for the GFRP pultruded beams, which shows a linear behaviour until failure. There is a non- linear response before the final failure for the beams with a/d ratios of. and.. This behaviour is possibly due to the crushing of the corners of the specimen at the support and at the loading points which leads to separation of the web flange junction. This progressive failure results in the web to continue carrying the applied load. The load carrying capacity of the beam is affected by the variation of the a/d ratio whereas a decreasing trend was observed with increasing a/d ratio. All the beams show a brittle failure in both flexural and transverse shear failure modes. Table presents a summary of the test results with respect to failure load, corresponding deflection and failure mode. Table. Summary of experimental results for GFRP beams Stress -strain behaviour. The strain measurements for the beams at the top and bottom faces in addition to the strain at the shear path are shown in Figures to. It can be seen that the tension strain at the bottom face is higher than the top face compression strain (i.e. for a/d ratio of and stress MPa the tension strain reaches 00 micro strain compared with 000 micro-strain in the compression side). There was a different trend in the strain on the top and bottom sides. The tension strains increased linearly up to failure, whereas the compression strains began to decrease non linearly as the load exceeded approximately % of the ultimate failure load. At the top side, the strain was negative demonstrating that the profile is compressed, as expected. With increasing load, however, the values tend to become positive indicating that the top surface is moving from being compressed to tensioned as shown in Figure. This behaviour reflects the onset of buckling considering that the flange can be assumed to be simply supported at the loading points. Consequently, the increase in the applied load increased the compression component of the moment which results in a local buckling of the flange. Figure 0 shows that the tensile strain decreases
13 Page of with decreasing shear span. The bottom side of the tested specimens were subjected to extensive tensile straining although failure cannot be observed there even after the compression region at the loading zone has failed entirely. Figure shows that shear strain increases with decreasing a/d due to the fact that a significant portion of the shear is transferred directly to the support by an inclined strut. As a result the amount of the direct load transfer increases with decreasing a/d ratio. In summary, the failure initiated at web flange junction and followed by buckling and/or crushing in the web depending on the a/d ratio: beams with higher a/d ratio experienced buckling failure whereas beams with lower a/d ratio experienced crushing. Figure. Load deflection curves for GFRP beams. Figure. Stress versus compression strain. Figure 0. Stress versus tensile strain. Figure. Stress versus shear strain. Failure mode. The different failure modes of the GFRP beams are shown in Figure. The observed failure modes can be classified as flexural failure and transverse shear failure. The shorter beams (a/d ratios of. and.) displayed progressive damage accumulation, which is indicated by the drops in the load deflection curves, with the increasing of the applied load. It was observed that the specimens had cracked and some twisted away from the centre towards one side. The mode of failure observed was transverse shear failure resulting in the delamination and cracking of the fibre along the edges of the pultruded beam in addition to local buckling on the compression flange as shown in Figures (a) and (b). Moreover, it was observed that the failure initiated at web-flange junctions and followed by premature buckling and crushing in the webs. This failure behaviour is described as a potential failure for pultruded GFRP sections under concentrated bearing load conditions. For beams with a/d ratios of. and, the failure occurred at the points of loading and distinct cracks 0
14 Page of developed on the top surface and side of the tubes. Furthermore, cracks developed at the intersection between the flange and the web due to the buckling, leading to separation between them. It was also observed that delamination crack happened at the compression surface and later progressed into the sides as a result of local buckling initiation as shown in Figure (c) and (d). Similar observation was reported by Guadeset al. and Kumaret al. in their investigations on the flexural behaviour of 00 and mm square pultruded FRP tubes. In their studies, however, they reported that the final failure of the specimen occurs mainly due to the effect of the local buckling of the thin wall which results in material delamination and cracking of the fibre along the edges of the beam under the point loads. Shear crack was not observed even for beams with the lowest a/d ratio. The possible reason for this is the presence of the ± o plies in addition to the main fibre on the tube which provides a stronger shear resistance along the transverse direction. Figure. Failure modes of GFRP beams for different shear span to depth ratios. Discussion Determination of elastic properties. Table gives a summary of the properties of the GFRP profiles based on the coupon and full scale tests. It can be seen from this table that there is a significant difference between the results determined from coupon and full scale tests. The main reason between the coupon and full scale results is the effect of discontinuity of the fibres (especially the + o ) in the small solid coupon of composite material. However, the continuity of the fibres in the full-scale beam results in higher effective elastic properties than the coupon specimens. Using these properties, the load-deflection behaviour of the full-scale pultruded GFRP beams were calculated using equation and compared with the experimental results. Figure displays comparison between the experimental and the predicted deflection calculated by using Timoshenko Beam Theory (equation ). Elastic properties obtained from full scale test (using BCM and SM) and coupon test have been used to predict the deflection.
15 Page of It can be seen that the Timoshenko Beam Theory provides a good approximation for the curves determined by the experimental tests. It can also be observed from the figure that using the elastic properties from BCM to calculate the beam deflection showed a good correlation with the experimental results for all a/d ratios. In contrast, analytical results using SM underestimated the experimental results and using coupon test results overestimated the deflection as shown in Figure. SM generally is relatively sensitive to the accuracy of the E measurement. When the span is short and for the same applied load, the deflection is in minimal. This observation is similar with Roberts and Al-Ubaidi wherein they indicated that the measured elastic properties of Pultruded FRP I-profile can change substantially depending on the sensitivity of the graphical method. Therefore, it can be concluded that the elastic properties (E and G) determined using the BCM can reliably predict the behaviour of full scale GFRP beams. Figure shows the relationship between the flexural and shear deflection percentage of total deflection as a function of a/d ratio. The flexural and shear deflection was calculated using the average value obtained in this study (E/G =.). It can be seen that the flexural deflection constitutes approximately 0% of the total deflection for a/d of.. In contrast, shear deflection was 0 % for the same a/d ratio. These observations reflect the significant contribution of shear deformation in the total deflection of beams with low shear span to depth ratio. From the figure it can also be observed that the percentage of shear deflection is less than 0% for a/d of 0 and a ratio of is required to decrease the shear deflection to less than %. Therefore, for composite beams with a/d equal or less than 0 the effect of shear deformation should be accounted in the total deflection calculation. Table. Summary of experimental properties for GFRP beams Figure. Comparison of theoretical and experimental deflection of beams with different a/d ratios.
16 Page of Figure. Contribution of flexural and shear deflection for beams with different a/d ratios. Effect of a/d ratio on shear stress. The effects of shear span to depth ratio on the shear stress of the GFRP beams were evaluated by calculating the shear stress experienced by the beams using equation : τ= where V is the shear force, Q is the first moment of area, I is the moment of inertia, and t is the wall thickness. The calculated values of shear stress at failure for different a/d ratios of the GFRP beams are shown in Figure. The results showed that the a/d ratio has a significant effect on the shear stress experienced by the pultruded GFRP beams. The reason is that the shorter span beams can be subjected to higher failure load which means higher shear force resulting in higher shear stress according to Equation. As a result, it can be seen that the shear stress increases with decreasing a/d ratio. Similar behaviour has been documented for composite sandwich beams and timber beams tested with different a/d ratios -. The authors indicated that shorter beam is subjected to a higher shear stress compared with longer span beams. They also mentioned that due to the core weakness, the shorter beams failed due to shear. In this study, no shear cracks were observed on the tested beams at the region of maximum shear even for short span beams. The relationship between the shear stress and the a/d ratios seems to be linear. Almost all the tested sections failed in similar mode by local buckling under the applied load followed by cracking at the compression side and the delamination of the plies. Although the tensile strain is low for small a/d ratios, the bottom face of the beam displays a crushing of fibres at the support without any failure at the mid-span as shown in Figure. The reason for this is the higher applied load corresponding to lower a/d ratio. ()
17 Page of The maximum calculated shear stress of the pultruded GFRP beams with shear span to depth ratio of. and are and MPa, respectively. These shear stresses are % and %, respectively, of the shear strength of the pultruded profile given in Table. These lower percentages indicated that the shear stress is not only the factor which affected the behaviour of the pultruded beams but also the flexural stress. Manaloet al. 0 mentioned that these combined stresses played an important part in understanding the overall behaviour of composites and should be considered in the design and analysis of composite materials. Figure. Shear stress versus shear span to depth ratio for GFRP beam. Effect of a/d ratio on flexural stress. The flexural behaviour of the GFRP hollow sections have been studied by calculating the bending stress using equation 0: σ= The calculated bending stresses for GFRP beams with different a/d ratios are shown in Figure. It can be seen that the bending stress increases with increasing a/d ratio. The maximum bending stress with a/d ratios of. and are and 00 MPa, respectively. These bending stress values are % and % of the compression strength, respectively, and % and %, respectively, of the tensile strength of the pultruded profile as mentioned in Table. This explains the reason why the failure is happening at the compression side. Furthermore, the results indicated that the specimen experiences considerable flexural stresses even at a/d ratio of. which contributed to the failure mechanisms. Similar result was reported by Turvey and Zhang in their investigation on the shear failure strength of web flange junctions in pultruded GRP profiles. In their study, however, they reported that failure is a function of (0) combined high shear and bending stresses at the interfaces of different plies. Figure. Bending stress versus shear span to depth ratio for GFRP beam.
18 Page of Effect of a/d ratio on failure mode. The GFRP pultruded beams showed a brittle failure mode. The failure happened without any reduction in the slope of the load deflection behaviour. The beams with a/d ratio of more than exhibited a flexural mode of failure. The failure of those beams was controlled by the buckling under the load points followed by cracks and delamination at the compression face in addition to a web flange junction failure as shown in Figures (c) and (d). The beams with a/d less than showed a transverse shear failure. This type of failure was resulting in the delamination and cracking of the fibre along the edges of the pultruded beam in addition to local buckling on the compression flange. This failure behaviour was reported by Turvey and Zhang and Wu and Bai as a web flange junction failure which caused mainly by the concentrated bearing load conditions. A change in the slope of the load deflection behaviour has been noticed. In some cases, it can be seen that there are some drops in the load at the failure progress stage for the beams with spans lower a/d ratios. This failure response is due to the progressive damage accumulation of the section. No pure shear failure or shear cracks appeared in all of the tested beams. The main reason for that is the stacking sequence of the plies of the GFRP pultruded sections are in the form of ± degrees. It was clearly noticed that the failure cracks position was closer to the top loading point than to the supports. Prediction of failure load for pultruded GFRP beams with different a/d ratio The contribution of the shear deformation was clearly observed for all a/d ratios considered in this study. Therefore, in order to estimate the failure load of the pultruded GFRP beams, it is important to account for the shear and the bending stresses in the prediction equation. Proposed prediction equation Based on the experimental results, buckling failure occurred at the concentrated load points and/or near the support locations. The main reason for this behaviour is the high shear forces
19 Page of that typically develop at those locations. Bank stated that, when the beam is subjected to high shear forces and high bending moment, the web is subjected to combined shear stress (τ) and axial compressive or tensile (flexural) stress,. As a result, the combined effect of both stresses is significant and should be accounted for in the prediction of failure load. Structural plastics design manual ASCE recommends using an interaction equation based on the isotropic plate theory to calculate the critical load which takes into account the combined effect of shear and flexural stresses. This equation expressed in the form: + () where and τ act are the actual flexural and shear stresses, respectively, and τ all are the corresponding material allowable stresses. In this formula the combined effect of the shear and flexure has been suggested and the failure load can be calculated using the following equation: = () In this study, a linear interaction equation similar to ASCE equation is proposed to predict the failure load of the pultruded GFRP beams which account for the combined effect of shear and flexure. In the proposed equation, buckling stress calculated according to Bank has been used instead of the allowable compressive strength due to the fact that almost all the tested hollow pultruded profiles failed with local buckling. Therefore, the predicted failure load of the pultruded GFRP beams can be calculated as: = () The allowable stresses of the pultruded GFRP material are listed in Table. Comparison between predicted and the experimental failure loads
20 Page of The predicted failure load of the pultruded GFRP beams tested using point load and the percentage difference between the predicted and actual (experimental) average failure loads are summarised in Table. For clarity, the comparison is also shown in Figure. It can be seen from Table and Figure that the proposed equation () shows a good agreement between the predicted and the actual failure load. For beam with a/d ratio., the proposed equation overestimates the failure load by %. This indicates that the beams are more likely to fail by transverse shear failure and the shear has the higher effect on the section s failure mode. In contrast, the flexural compression stress is the more dominant stress to cause the failure for pultruded beams with a/d ratios of.. Moreover, it can be clearly noticed that the use of equation () to predict the failure load depends on the ultimate flexural stress will overestimate the failure load by as much as to %. Figure shows the percentages of stress contribution from the failure stress of the pultruded beams. As seen from the figure, for beams of a/d ratio., shear stress contribution (%) for the failure load is higher than that for the flexural stress (%). For beams with higher a/d ratio, the flexural stress becomes the dominant stress to cause the failure with % of the failure load compared with % of shear stress, respectively. These percentages showed that the predicted contributions compare well with the experimental contributions for shear and flexural stresses. In general, the proposed equation provided a conservative but practical estimation of the failure load of the pultruded GFRP beams with different a/d ratios. Table. Predicted failure load compared with the actual failure load Figure. Comparison between the predicted and the actual failure loads. Figure. Percentages of stress contribution from the total failure stress. Conclusions
21 Page of The behaviour of GFRP pultruded square beams with different shear span to depth (a/d) ratios was investigated using the four-point bending test. Similarly, the elastic properties of the beams were determined by testing full-scale specimens. The following conclusions can be drawn based on the results of the investigation:. The back calculation method gives more reliable values of effective flexural and shear moduli of pultruded hollow GFRP square sections compared with simultaneous method and coupon test. This method is based on the Bernoulli equation and uses the strain readings at mid-span of the beam. A good correlation between the predicted and the actual load-deflection behaviour was achieved using the elastic properties determined from this method.. The shear deformation contributes by as much as 0% to the total deflection of beams with low a/d ratio. Thus, it is recommended to account for the shear deflection in the deflection calculation of GFRP beams when (a/d) is less than or equal to.. The shear stress experienced by the beam decreases with increasing a/d. In contrast, the flexural stress increases with increasing a/d ratio.. The failure of the beam is governed by the buckling under the loading points followed by cracks and delamination at the web-flange junction at the compression face.. The proposed equation accounting for the combined effect of shear and flexural stresses in pultruded GFRP square beams and accounting for the buckling stress of composites reasonably predicted the failure load of full size pultruded GFRP beams.. Aside from shear and flexural stresses, it was found that there is a complexity on the overall behaviour of pultruded GFRP square beams with low a/d, which needs further investigation. Acknowledgement
22 Page of The authors would like to acknowledge the support of Wagner s Composite Fibre Technologies (WCFT) for providing the GFRP pultruded sections. The first author would like to acknowledge the financial support by the Ministry of Higher Education and Scientific Research-Iraq. References. Bakis C, Bank LC, Brown V, et al. Fiber-reinforced polymer composites for construction-state-ofthe-art review. Journal of Composites for Construction. 0; : -.. Hollaway L. A review of the present and future utilisation of FRP composites in the civil infrastructure with reference to their important in-service properties. Construction and Building Materials. 0; : -.. Bank LC. Shear coefficients for thin-walled composite beams. Composite Structures. ; : -.. Barbero EJ, Fu S-H and Raftoyiannis I. Ultimate bending strength of composite beams. Journal of Materials in Civil Engineering. ; : -0.. Omidvar B. Shear coefficient in orthotropic thin-walled composite beams. Journal of Composites for Construction. ; : -.. Nagaraj V and GangaRao HV. Static behavior of pultruded GFRP beams. Journal of Composites for Construction. ; : 0-.. Bank LC. Composite for Construction Structural Design with FRP Materials. New Jersey: Jone Wiley & Sons, 0, p... Davalos JF, Salim H, Qiao P, Lopez-Anido R and Barbero E. Analysis and design of pultruded FRP shapes under bending. Composites Part B: Engineering. ; : -0.. Roberts T and Masri H. Section properties and buckling behavior of pultruded FRP profiles. Journal of reinforced plastics and composites. 0; : Manalo A, Mutsuyoshi H and Matsui T. Testing and characterization of thick hybrid fibre composites laminates. International Journal of Mechanical Sciences. ; : -0.. Cardoso D, Harries K and Batista E. On the Determination of Mechanical Properties for Pultruded GFRP Sections. International Conference on FRP composites in Civil Engineering. Vancouver, Canada: Internationl Institute for FRP in Construction.. Guades E, Aravinthan T and Islam MM. Characterisation of the mechanical properties of pultruded fibre-reinforced polymer tube. Materials & Design. ; : 0-.. Bank LC. Flexural and shear moduli of full-section fiber reinforced plastic(frp) pultruded beams. Journal of Testing and Evaluation. ; : 0-.. Neto A and Rovere H. Flexural stiffness characterization of fiber reinforced plastic (FRP) pultruded beams. Composite structures. 0; : -.. Mottram J. Shear modulus of standard pultruded fiber reinforced plastic material. Journal of Composites for Construction. 0; : -.. Chambers RE. ASCE design standard for pultruded fiber-reinforced-plastic (FRP) structures. Journal of Composites for Construction. ; : -.. Parke G and Hewson N. ICE manual of bridge engineering. history. 0; :.. ISO. Textile-glass-reinforced plastics, prepegs, moulding compounds and laminates: Determination of the textile-glass and mineral-filler content- Calcination methods... ASTM D. ASTM D/DM-0 Standard practice for determine sandwich beam flexural and shear stiffeness. West Conshohocken, (PA): ASTM International, 0.. Hayes M and Lesko J. The effect of non-classical behaviors on the measurement of the Timoshenko shear stiffness. Proc nd Inter Conf FRP Composites in Civil Engineering CICE. 0, p. -0.
23 Page of Wu C and Bai Y. Web crippling behaviour of pultruded glass fibre reinforced polymer sections. Composite Structures. ; 0: Kumar P, Chandrashekhara K and Nanni A. Structural performance of a FRP bridge deck. Construction and Building Materials. 0; : -.. Roberts T and Al-Ubaidi H. Flexural and torsional properties of pultruded fiber reinforced plastic I-profiles. Journal of Composites for Construction. 0; : -.. Dai J and Hahn HT. Flexural behavior of sandwich beams fabricated by vacuum-assisted resin transfer molding. Composite Structures. 0; : -.. Yoshihara H and Furushima T. Shear strengths of wood measured by various short beam shear test methods. Wood science and technology. 0; : -.. Awad ZK, Aravinthan T and Manalo A. Geometry effect on the behaviour of single and gluelaminated glass fibre reinforced polymer composite sandwich beams loaded in four-point bending. Materials & Design. ; : -0.. Turvey GJ and Zhang Y. Shear failure strength of web flange junctions in pultruded GRP WF profiles. Construction and Building Materials. 0; : -.. ASCE. Structural Plastics Design Manual. ASCE Manuals and Reports on Engineering Practice. Reston, VA: American Society of Civil Engineering,.
24 Page of *All dimensions are in mm as per Table mm All Figures Figure. Experimental set-up for characterisation of elastic properties P mm a 00 mm a L *All dimensions are in mm as per Table Figure. Experimental setup for the behaviour of GFRP beams Figure. Load deflection relationship for GFRP beams
25 Page of Figure. Elastic modulus (E) and shear stiffness (KGA) versus Load for a/d =. Figure. Flexural modulus (E) and shear stiffness (KGA) versus Load for a/d =. Figure. Flexural modulus (E) and shear stiffness (KGA) versus Load for a/d =.
26 Page of Figure. Typical graph to determine E and KG using SM Figure. Load deflection curves for GFRP beams Figure. Stress versus compression strain
27 Page of Figure 0. Stress versus tensile strain Figure. Stress versus shear strain
28 Page of (a) a/d=. (c) a/d=. (d) a/d= Figure. Failure modes of GFRP beams for different shear span to depth ratios Figure. Comparison of theoretical and experimental deflection of beams with different a/d ratios
29 Page of Figure. Contribution of flexural and shear deflection for beams with different a/d ratios Figure. Shear stress versus shear span to depth ratio for GFRP beam Figure. Bending stress versus shear span to depth ratio for GFRP beam
30 Page of Figure. Comparison between the predicted and the actual failure loads Figure. Percentages of stress contribution from the total failure stress
31 Page 0 of All Tables Table. Mechanical properties from coupon test Properties Average value SD Compressive modulus (Longitudinal), GPa. Compressive strength, MPa 0 Tensile modulus (Longitudinal), GPa Tensile Strength (MPa) Flexural modulus (Longitudinal) (GPa).. Shear modulus (Longitudinal) (GPa). 0. Shear Strength (MPa) 0 Inter-laminar shear strength (MPa) Table. Details of the specimens tested for the elastic properties Span length mm Shear span, a mm a/d Table. Details of the specimens tested for the behaviour of GFRP beams Span length mm Shear span, a mm a/d Table. Summary of average E and KGA for each span for GFRP beam testing (BCM) a/d E GPa C.O.V % KGA GPa-cm C.O.V % G GPa Ave..
32 Page of Table. Summary of experimental results for GFRP beams Shear span/ depth Average failure load Deflection Failure mode kn mm. TS TS: transverse shear failure F: flexural failure. TS. 0. F 0. F Table. Summary of experimental properties for GFRP beams Test type E modulus GPa G modulus GPa Coupon.. BCM. SM.. Table. Predicted failure load compared with the actual failure load a/d ratio Exp. kn Eq. kn Eq. kn
Sensors 2012, 12, 16024-16036; doi:10.3390/s121216024 Article OPEN ACCESS sensors ISSN 1424-8220 www.mdpi.com/journal/sensors Determination of the Shear Buckling Load of a Large Polymer Composite I-Section
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., firstname.lastname@example.org Faculdade de Tecnologia de São Paulo, FATEC-SP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
DETERMINATION OF EI FOR PULTRUDED GFRP SHEET PILE PANELS Yixin Shao, Cynthia Giroux and Zeid Bdeir McGill University Montreal, Quebec, Canada Abstract The flexural rigidity, EI, plays an especially important
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
01/02/2016 Marco Donà Finite Element Modelling with Plastic Hinges 1 Plastic hinge approach A plastic hinge represents a concentrated post-yield behaviour in one or more degrees of freedom. Hinges only
Unit III Theory of columns 1 Unit III Theory of Columns References: Punmia B.C.,"Theory of Structures" (SMTS) Vol II, Laxmi Publishing Pvt Ltd, New Delhi 2004. Rattan.S.S., "Strength of Materials", Tata
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED - PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
6 th International Conference on Advances in Experimental Structural Engineering 11 th International Workshop on Advanced Smart Materials and Smart Structures Technology August 1-2, 2015, University of
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
DETERMINATION OF DUCTILITY CAPACITY AND OTHER SECTION PROPERTIES OF T-SHAPED RC WALLS IN DIRECT DISPLACEMENT-BASED DESIGN E. Smyrou 1, T.J. Sullivan 2, M.J.N. Priestley 3 and G.M. Calvi 4 1 PhD Candidate,
TESTING AND ANALYSIS OF COMPOSITE SANDWICH BEAMS I. M. Daniel, J. L. Abot, and K. A. Wang Walter P. Murphy Professor, Departments of Civil and Mechanical Engineering, Robert R. McCormick School of Engineering
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
16 PLATE GIRDERS II 1.0 INTRODUCTION This chapter describes the current practice for the design of plate girders adopting meaningful simplifications of the equations derived in the chapter on Plate Girders
VOL. 5, NO. 4, APRIL 010 ISSN 1819-6608 006-010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kip-in.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 16-17 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
7 TRANSVERSE SHEAR Before we develop a relationship that describes the shear-stress distribution over the cross section of a beam, we will make some preliminary remarks regarding the way shear acts within
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, two-dimensional structural components of which
INSTITUTE OF AERONAUTICAL ENGINEERING (Autonomous) Dundigal, Hyderabad -00 04 CIVIL ENGINEERING QUESTION BANK Course Name : STRENGTH OF MATERIALS II Course Code : A404 Class : II B. Tech II Semester Section
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & Free-Body Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
Example on Design of Slab Bridge Design Data and Specifications Chapter 5 SUPERSTRUCTURES Superstructure consists of 10m slab, 36m box girder and 10m T-girder all simply supported. Only the design of Slab
Seismic Pushover Analysis Using AASHTO Guide Specifications for LRFD Seismic Bridge Design Elmer E. Marx, Alaska Department of Transportation and Public Facilities Michael Keever, California Department
A Study on the Tube of Integral Propeller Shaft for the Rear-wheel Drive Automobile Using Carbon Composite Fiber Kibong Han Mechatronics Department, Jungwon University, 85 Munmu-ro, Goesan-gun, South Korea.
www.ijaser.com 2012 by the authors Licensee IJASER- Under Creative Commons License 3.0 email@example.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angle-ply FRP laminates
CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach - Fifth Edition Fifth Edition SERVICEABILITY OF BEAMS AND ONE-WAY SLABS A. J. Clark School of Engineering Department of Civil
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
OPTI Buckling Buckling and Stability: As we learned in the previous lectures, structures may fail in a variety of ways, depending on the materials, load and support conditions. We had two primary concerns:
METNET Workshop October 11-12, 2009, Poznań, Poland Experimental and numerical analysis of sandwich metal panels Zbigniew Pozorski, Monika Chuda-Kowalska, Robert Studziński, Andrzej Garstecki Poznan University
CHAPTER 6: ULTIMATE LIMIT STATE 6.1 GENERAL It shall be in accordance with JSCE Standard Specification (Design), 6.1. The collapse mechanism in statically indeterminate structures shall not be considered.
TRANSVERSE PLATE-TO-SQUARE/RECTANGULAR HSS CONNECTIONS by Jeffrey A. Packer 1 1 Bahen/Tanenbaum Professor of Civil Engineering, University of Toronto, Ontario, Canada Some of the common types of plate-to-rectangular
ENGINEERING SCIENCE H1 OUTCOME 1 - TUTORIAL COLUMNS EDEXCEL HNC/D ENGINEERING SCIENCE LEVEL H1 FORMERLY UNIT 21718P This material is duplicated in the Mechanical Principles module H2 and those studying
ENCE 455 Design of Steel Structures III. Compression Members C. C. Fu, Ph.D., P.E. Civil and Environmental Engineering Department University of Maryland Compression Members Following subjects are covered:
Journal of Marine Science and Technology, Vol., No., pp. -8 () MODELING THE EFFECTIVE ELASTIC MODULUS OF RC BEAMS EXPOSED TO FIRE Jui-Hsiang Hsu*, ***, Cherng-Shing Lin**, and Chang-Bin Huang*** Key words:
Formulation of Equivalent Steel Section for Partially Encased Composite Column under Concentric Gravity Loading Debaroti Ghosh & Mahbuba Begum Dept of Civil Engineering, Bangladesh University of Engineering
Static and Time Dependent Failure of Fibre Reinforced Elastomeric Components Salim Mirza Element Materials Technology Hitchin, UK Introduction Fibre reinforced elastomers are used in many applications,
Introduction to Steel Design, Tensile Steel Members Modes of Failure & Effective Areas MORGAN STATE UNIVERSITY SCHOOL OF ARCHITECTURE AND PLANNING LECTURE VIII Dr. Jason E. Charalambides Failure in Flexure!
Delamination Studies in Fibre-Reinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
Materials How materials work Compression Tension Bending Torsion Elemental material atoms: A. Composition a) Nucleus: protons (+), neutrons (0) b) Electrons (-) B. Neutral charge, i.e., # electrons = #
An Integrated Thermomechanical Method for Modeling Fiber Reinforced Polymer Composite Structures in Fire Ziqing Yu¹ and Aixi Zhou² ¹Department of Engineering Technology, University of North Carolina at
Jordan Journal of Civil Engineering, Volume 8, No. 2, 214 Prediction of Compressive Strength of Fibrous Composites Using Two Different Approaches Yousef S. Al Rjoub 1) * and Karim S. Numayr 2) 1) Civil
STRENGTH AND STIFFNESS REDUCTION OF LARGE NOTCHED BEAMS By Joseph F. Murphy 1 ABSTRACT: Four large glulam beams with notches on the tension side were tested for strength and stiffness. Using either bending
CH. 4 BEAMS & COLUMNS BEAMS Beams Basic theory of bending: internal resisting moment at any point in a beam must equal the bending moments produced by the external loads on the beam Rx = Cc + Tt - If the
MODELING SLAB-COLUMN CONNECTIONS REINFORCED WITH GFRP UNDER LOCALIZED IMPACT QI ZHANG and AMGAD HUSSEIN Faculty of Engineering, Memorial University of Newfoundland St. John s, Newfoundland, Canada, A1B
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 79-85 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto Gutierrez-Miravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
Peak Strain and Displacement Sensors for Structural Health Monitoring AKIRA MITA and SHINPEI TAKAHIRA ABSTRACT Simple and inexpensive passive sensors that can monitor the peak strain or displacement of
STRUCTURAL MECHANICS: CE203 Chapter 5 Torsion Notes are based on Mechanics of Materials: by R. C. Hibbeler, 7th Edition, Pearson Dr B. Achour & Dr Eng. K. El-kashif Civil Engineering Department, University
Chapter 4 Deflection and Stiffness 1 2 Chapter Outline Spring Rates Tension, Compression, and Torsion Deflection Due to Bending Beam Deflection Methods Beam Deflections by Superposition Strain Energy Castigliano
MECHANICS OF MATERIALS Prepared by Engr. John Paul Timola Mechanics of materials branch of mechanics that studies the internal effects of stress and strain in a solid body. stress is associated with the
SP-230 57 Strain-Based Design Model for FRP-Confined Concrete Columns by N. Saenz and C.P. Pantelides Synopsis: A constitutive strain-based confinement model is developed herein for circular concrete columns
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6-13-1, Ohsawa, Mitaka,
Failure interaction curves for combined loading involving torsion, bending, and axial loading W M Onsongo Many modern concrete structures such as elevated guideways are subjected to combined bending, torsion,
Fundamentals of Structural Design Part of Steel Structures Civil Engineering for Bachelors 133FSTD Teacher: Zdeněk Sokol Office number: B619 1 Syllabus of lectures 1. Introduction, history of steel structures,
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stress-strain diagram
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, firstname.lastname@example.org
Chapter 5 Elastic Strain, Deflection, and Stability Elastic Stress-Strain Relationship A stress in the x-direction causes a strain in the x-direction by σ x also causes a strain in the y-direction & z-direction
International Journal of Civil Structural 6 Environmental And Infrastructure Engineering Research Vol.1, Issue.1 (2011) 1-15 TJPRC Pvt. Ltd.,. INFLUENCE OF FLANGE STIFFNESS ON DUCTILITY BEHAVIOUR OF PLATE
Local Stresses in Belt Turnovers in Conveyor Belt By: Conveyor Dynamics, Inc. personnel Conveyor Dynamics, Inc. 1111 W. Holly Street, Suite A Bellingham, WA 985 USA Abstract Belt turnovers are commonly
Powder Metallurgy Progress, Vol.3 (003), No 3 119 THE DETERMINATION OF FRACTURE STRENGTH FROM ULTIMATE TENSILE AND TRANSVERSE RUPTURE STRESSES A.S. Wronski, A.Cias Abstract It is well-recognized that the
EXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS Kevin L. Peil +, Ever J. Barbero +, Eduardo M. Sosa* + Department of Mechanical and Aerospace Engineering, West Virginia University (WVU), Morgantown,
(130) CHAPTER 6: Shearing Stresses in Beams When a beam is in pure bending, the only stress resultants are the bending moments and the only stresses are the normal stresses acting on the cross sections.
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a cross-sectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
N. Kishi, E-89, 1/8 A PROPOSAL OF DESIGN PROCEDURE FOR FLEXURAL STRENGTHENING RC BEAMS WITH FRP SHEET Yusuke Kurihashi Norimitsu Kishi Hiroshi Mikami Sumiyuki Sawada Civil Engrg. Research Muroran Inst.
UNIVERSITÀ DEGLI STUDI DI PADOVA DIPARTIMENTO DI INGEGNERIA CIVILE, EDILE ED AMBIENTALE CORSO DI LAUREA MAGISTRALE IN INGEGNERIA CIVILE Tesi di laurea Magistrale in Ingegneria Civile Curriculum Strutture
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER -6- BENDING Part -1-1 CHAPTER -6- Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
MME445: Lecture 27 Materials and Shape Part 1: Materials for efficient structure A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Learning Objectives Knowledge & Understanding Understand the
Technical Report Title: Document ID: Authors: Supplementary Uniaxial Compressive Strength Testing of DGR-3 and DGR-4 Core TR-08-39 B. Gorski, T. Anderson and D. Rodgers CANMET Mining and Mineral Sciences
CIE309 : PLASTICITY THEME IS FIRST OCCURANCE OF YIELDING THE LIMIT? M M - N N + + σ = σ = + f f BENDING EXTENSION Ir J.W. Welleman page nr 0 kn Normal conditions during the life time WHAT HAPPENS DUE TO
EFFECT OF SHEAR REINFORCEMENT ON FAILURE MODE OF RC BRIDGE PIERS SUBJECTED TO STRONG EARTHQUAKE MOTIONS Atsuhiko MACHIDA And Khairy H ABDELKAREEM SUMMARY Nonlinear D FEM was utilized to carry out inelastic
Stress-Strain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
Modes of Loading (1) tension (a) (2) compression (b) (3) bending (c) (4) torsion (d) and combinations of them (e) Figure 4.2 1 Standard Solution to Elastic Problems Three common modes of loading: (a) tie
University of South Florida Scholar Commons Graduate Theses and Dissertations Graduate School 003 A study of the critical condition of a battened column and a frame by classical methods Jamal A.H Bekdache
Task 1 - Material Testing of Bionax Pipe and Joints Submitted to: Jeff Phillips Western Regional Engineer IPEX Management, Inc. 20460 Duncan Way Langley, BC, Canada V3A 7A3 Ph: 604-534-8631 Fax: 604-534-7616